FOR SOLIDS AND LIQUIDS. 



155 



Alloy. 



Specific Gravity. 



Authority. 



silver and tin — con- 

 tinued. 



Ag Sn 3 ^ 7.936, 19°.3. 



Ag Sn 5 : 7.551, 18°.8. 



Ag Sn 6 7.666, 18°.4. 



Ag Sn 18 ! 7 - 421 > 18 °- 6 - 



«ILV£R AXD LEAD. 



Ag 4 Pb I 10.800, 13°.5__. 



Ag 2 Pb 10.925, 13°.8__. 



AgPb ! 10.054, 12°.5__. 



Ag Pbj ! 11.144, 18°.2__. 



AgPb 4 



AgPb 10 



AgPb 25 



Holzraann. P. T. 1860, 177. 



Matthiessen. P. T. 1860, 177. 



SILVER AND COPPER.* 



11.196,21° 



11.285, 22°.2 



11.334, 20°. 6 



Ag s Cu 2 9.9045 __ 



" Solid 9.9045 | 



" Molten j 9.0554 j 



GOLD AND TIN. 



Au 4 Sn 16.367, 15°.4_ 



Au„ Sn 14.244, 14 D .2_ 



AuSn I 11.833, 14°.6_ 



Au 2 Sn s i 10.794, 23°. 6. 



Au Sn, I 10.168, 23°.7_ 



Levol. J. 5, 768. 

 Koberts. C. N. 31, 143. 



Holzmann. P. T. 1860, 177. 



Au 2 Sn 5 



Au Sn 3 __. 

 Au Sn 4 ___ 



Au Sn 6 



Au Sn 9 



Au Sn 15 __. 

 Au Sn m __. 



GOLD AND LEAD. 



Au 4 Pb. 

 Au., Pb. 

 AuPb- 

 Au Pb.,. 

 Au Pb 3 . 

 Au Pb 4 . 

 Au Pb 5 . 

 Au Pb, n 



GOLD AND BISMUTH. 



9.715, 22°. 4. 

 9.405, 23°.7. 

 8.931, 25°.6. 

 8.470, 23°. 1. 

 8.118, 22°.4_ 

 7.801, 22°. 8. 

 7.441, 22°.9_ 



17.013, 14°.3_ 

 15.603, 14°.5_ 

 14.466, 14°.3_ 

 13.306, 22°. 1. 



12.737, 21°. 3. 

 12.445, 21°.6. 

 12.274, 19°.4_ 

 11.841,2:; -.3. 



Ail, Bi 

 AuBi. 

 Au Bi, 

 Au Bi, 



14.844,16° _. 

 13.403, 16°.5. 

 12.067, 16__. 

 11.025,23° _. 



Matthiessen. P. T. 1860, 177. 



Holzmonn. P. T. 1860, 177. 



* See Karmarsch. Beiblatier 2, 194, for feixteen Ag Cu alloys. 



